IIIE SECTION A MANUFACTURING TECHNOLOGY NOTES : 10.CASTINGS AND ITS DEFECTS
Castings defects and Inspection
A casting defect is an irregularity in the metal casting process that is undesired. Some
defects can be tolerated while others can be repaired otherwise they must be eliminated.
They are broken down into five main categories:
Mold material defects,
Pouring metal defects, and
Shrinkage defects occur when feed metal is not available to compensate for
shrinkage as the metal solidifies.
Shrinkage defects can be split into two different types:
Open shrinkage defects and closed shrinkage defects.
Open shrinkage defects are open to the atmosphere, therefore as the shrinkage cavity
forms air compensates.
There are two types of open air defects: pipes and caved surfaces. Pipes form at the
surface of the casting and burrow into the casting, while caved surfaces are shallow
cavities that form across the surface of the casting
Closed shrinkage defects, also known as shrinkage porosity, are defects that form within
the casting. Isolated pools of liquid form inside solidified metal, which are called hot
spots. The shrinkage defect usually forms at the top of the hot spots. They require a
nucleation point, so impurities and dissolved gas can induce closed shrinkage defects.
The defects are broken up into macro porosity and microporosity (or microshrinkage),
where macroporosity can be seen by the naked eye and microporosity cannot
Gas porosity is the formation of bubbles within the casting after it has cooled. This
occurs because most liquid materials can hold a large amount of dissolved gas, but the
solid form of the same material cannot, so the gas forms bubbles within the material as it
cools. Gas porosity may present itself on the surface of the casting as porosity or the pore
may be trapped inside the metal which reduces strength in that vicinity.
Pouring Metal defects Pouring metal defects include misruns, cold shuts, and
inclusions. A misrun occurs when the liquid metal does not completely fill the mold
cavity, leaving an unfilled portion. Cold shuts occur when two fronts of liquid metal do
not fuse properly in the mold cavity, leaving a weak spot. Both are caused by either a
lack of fluidity in the molten metal or cross-sections that are too narrow.
There are two defects in this category: hot tears and hot spots. Hot tears, also known as
hot cracking, are failures in the casting that occur as the casting cools. This
happens because the metal is weak when it is hot and the residual stresses in the
material can cause the casting to fail as it cools. Proper mold design prevents this
type of defect.
Hot spots are areas on the surface of casting that become very hard because they cooled
more quickly than the surrounding material. This type of defect can be avoided by proper
cooling practices or by changing the chemical composition of the metal.[
Mold material defects :
In die casting the most common defects are misruns and cold shuts. These defects can be
caused by cold dies, low metal temperature, dirty metal, lack of venting, or too much
lubricant. Other possible defects are gas porosity, shrinkage porosity, hot tears, and flow
marks. Flow marks are marks left on the surface of the casting due to poor gating, sharp
corners, or excessive lubricant.
A longitudinal facial crack is a specialized type of defect that only occurs in continuous
casting processes. This defect is caused by uneven cooling, both primary cooling and
secondary cooling, and includes molten steel qualities, such as the chemical composition
being out of specification, cleanliness of the material, and homogeneity
Sand castings :
Sand casting has many defects that can occur due to the mold failing. The mold usually
fails because of one of two reasons: the wrong material is used or it is improperly
The first type is mold erosion, which is the wearing away of the mold as the liquid metal
fills the mold. This type of defect usually only occurs in sand castings because most other
casting processes have more robust molds. The castings produced have rough spots and
excess material. The molding sand becomes incorporated into the casting metal and
decreases the ductility, fatigue strength, and fracture toughness of the casting. This can be
caused by a sand with too little strength or a pouring velocity that is too fast. The pouring
velocity can be reduced by redesigning the gating system to use larger runners or multiple
gates.A related source of defects are drops, in which part of the molding sand from the
cope drops into the casting while it is still a liquid. This also occurs when the mold is not
The second type of defect is metal penetration, which is when the liquid metal penetrates
into the molding sand. This causes a rough surface finish. This caused by sand particles
that are too coarse, lack of mold wash, or pouring temperatures that are too high.
If the pouring temperature is too high or a sand of low melting point is used then the sand
can fuse to the casting. When this happens the surface of the casting produced has a
brittle, glassy appearance.
A run out is when the liquid metal leaks out of the mold because of a faulty mold or
Scabs are a thin layer of metal that sits proud of the casting. They are easy to remove and
always reveal a buckle underneath, which is an indentation in the casting surface. Rattails
are similar to buckles, except they are thin line indentations and not associated with
scabs. Another similar defect is a pulldowns, which are buckles that occur in the cope of
sand castings. All of these defects are visual in nature and no reason to scrap the
workpiece. These defects are caused by overly high pouring temperatures or deficiencies
of carbonaceous material.
A swell occurs when the mold wall gives way across a whole face, and is caused by an
improperly rammed mold.
Burn-on occurs when metallic oxides interact with impurities in silica sands. The result is
sand particles embedded in the surface of the finished casting. This defect can be avoided
by reducing the temperature of the liquid metal, by using a mold wash, and by using
various additives in the sand mixture.
1. Visual examinations: depends on the skill and experience of
the inspector to locate defects.
2. Sound or percussion tests : It is used for relatively large
discontinuities in homogeneous metal casting of simple shape
and uniform cross sections
3. Impact test : It is a descructive test
4. Pressure test It is used to locate leaks and test overall
5. Magnetic and flouroscent powder inspection : The test
used to locate exact location and type of flaw in iron and
steel and magnetic alloys.
6. Radio graphic and x ray examination : It can be used for
inspecting castings of any metal
7. Electrical conductivity method : It is limited only to
uniform sectional thickness and metalargical structures.
8. Penetrants inspection tecqnicqs : It is used for small cracks
in castings which cant be detected by naked eye and also
reveling those surface defects which cannt be detected
9. Ultrasonic testing : It is used to detect the defects of
dimensions of castings very accurately and quickly.
10 .Test are also performed to check dimensional
accuracy,surface finish,chemical analysis, mettalographic
test and mechanical tests like tensile test, bend and notch
bend tests and hardness tests.